General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 7.96 - 8 g/cm³ Show Material materials with Density of 7.96 - 8 g/cm³ |

50.0 °C | 7.95 g/cm³ Show Material materials with Density of 7.95 g/cm³ | |

100.0 °C | 7.93 g/cm³ Show Material materials with Density of 7.93 g/cm³ | |

150.0 °C | 7.9 g/cm³ Show Material materials with Density of 7.9 g/cm³ | |

200.0 °C | 7.88 g/cm³ Show Material materials with Density of 7.88 g/cm³ | |

250.0 °C | 7.86 g/cm³ Show Material materials with Density of 7.86 g/cm³ | |

300.0 °C | 7.84 g/cm³ Show Material materials with Density of 7.84 g/cm³ | |

350.0 °C | 7.82 g/cm³ Show Material materials with Density of 7.82 g/cm³ | |

400.0 °C | 7.79 g/cm³ Show Material materials with Density of 7.79 g/cm³ | |

450.0 °C | 7.77 g/cm³ Show Material materials with Density of 7.77 g/cm³ | |

500.0 °C | 7.75 g/cm³ Show Material materials with Density of 7.75 g/cm³ | |

550.0 °C | 7.72 g/cm³ Show Material materials with Density of 7.72 g/cm³ | |

600.0 °C | 7.7 g/cm³ Show Material materials with Density of 7.7 g/cm³ | |

650.0 °C | 7.67 g/cm³ Show Material materials with Density of 7.67 g/cm³ | |

700.0 °C | 7.65 g/cm³ Show Material materials with Density of 7.65 g/cm³ | |

750.0 °C | 7.62 g/cm³ Show Material materials with Density of 7.62 g/cm³ | |

800.0 °C | 7.6 g/cm³ Show Material materials with Density of 7.6 g/cm³ | |

Mechanical

Property | Temperature | Value |
---|---|---|

Elastic modulus | -100.0 °C | 206 GPa Show Material materials with Elastic modulus of 206 GPa |

20.0 °C | 196 - 198 GPa Show Material materials with Elastic modulus of 196 - 198 GPa | |

50.0 °C | 194.83 GPa Show Material materials with Elastic modulus of 194.83 GPa | |

100.0 °C | 190 - 192 GPa Show Material materials with Elastic modulus of 190 - 192 GPa | |

150.0 °C | 186.88 GPa Show Material materials with Elastic modulus of 186.88 GPa | |

200.0 °C | 182 - 183 GPa Show Material materials with Elastic modulus of 182 - 183 GPa | |

250.0 °C | 178.44 GPa Show Material materials with Elastic modulus of 178.44 GPa | |

300.0 °C | 174 - 175 GPa Show Material materials with Elastic modulus of 174 - 175 GPa | |

350.0 °C | 169.81 GPa Show Material materials with Elastic modulus of 169.81 GPa | |

400.0 °C | 165.69 - 167 GPa Show Material materials with Elastic modulus of 165.69 - 167 GPa | |

450.0 °C | 161.57 GPa Show Material materials with Elastic modulus of 161.57 GPa | |

500.0 °C | 157.45 - 159 GPa Show Material materials with Elastic modulus of 157.45 - 159 GPa | |

550.0 °C | 153.43 GPa Show Material materials with Elastic modulus of 153.43 GPa | |

600.0 °C | 149.5 - 150 GPa Show Material materials with Elastic modulus of 149.5 - 150 GPa | |

650.0 °C | 145.58 GPa Show Material materials with Elastic modulus of 145.58 GPa | |

700.0 °C | 141.66 - 142 GPa Show Material materials with Elastic modulus of 141.66 - 142 GPa | |

750.0 °C | 138.03 GPa Show Material materials with Elastic modulus of 138.03 GPa | |

800.0 °C | 134 - 134.3 GPa Show Material materials with Elastic modulus of 134 - 134.3 GPa | |

900.0 °C | 127 GPa Show Material materials with Elastic modulus of 127 GPa | |

1000.0 °C | 120 GPa Show Material materials with Elastic modulus of 120 GPa | |

Unlock all property charts | ||

Elongation | 20.0 °C | 30 % Show Material materials with Elongation of 30 % |

Elongation, transverse | 20.0 °C | 20 % Show Material materials with Elongation, transverse of 20 % |

Poisson's ratio | 20.0 °C | 0.28 [-] Show Material materials with Poisson's ratio of 0.28 [-] |

50.0 °C | 0.28 [-] Show Material materials with Poisson's ratio of 0.28 [-] | |

100.0 °C | 0.28 [-] Show Material materials with Poisson's ratio of 0.28 [-] | |

150.0 °C | 0.28 [-] Show Material materials with Poisson's ratio of 0.28 [-] | |

200.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | |

250.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | |

300.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | |

350.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | |

400.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | |

450.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | |

500.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | |

550.0 °C | 0.31 [-] Show Material materials with Poisson's ratio of 0.31 [-] | |

600.0 °C | 0.31 [-] Show Material materials with Poisson's ratio of 0.31 [-] | |

650.0 °C | 0.31 [-] Show Material materials with Poisson's ratio of 0.31 [-] | |

700.0 °C | 0.32 [-] Show Material materials with Poisson's ratio of 0.32 [-] | |

750.0 °C | 0.32 [-] Show Material materials with Poisson's ratio of 0.32 [-] | |

800.0 °C | 0.32 [-] Show Material materials with Poisson's ratio of 0.32 [-] | |

Unlock all property charts | ||

Shear modulus | 20.0 °C | 77.01 GPa Show Material materials with Shear modulus of 77.01 GPa |

50.0 °C | 76.13 GPa Show Material materials with Shear modulus of 76.13 GPa | |

100.0 °C | 74.56 GPa Show Material materials with Shear modulus of 74.56 GPa | |

150.0 °C | 72.79 GPa Show Material materials with Shear modulus of 72.79 GPa | |

200.0 °C | 71.02 GPa Show Material materials with Shear modulus of 71.02 GPa | |

250.0 °C | 69.26 GPa Show Material materials with Shear modulus of 69.26 GPa | |

300.0 °C | 67.39 GPa Show Material materials with Shear modulus of 67.39 GPa | |

350.0 °C | 65.63 GPa Show Material materials with Shear modulus of 65.63 GPa | |

400.0 °C | 63.86 GPa Show Material materials with Shear modulus of 63.86 GPa | |

450.0 °C | 62.1 GPa Show Material materials with Shear modulus of 62.1 GPa | |

500.0 °C | 60.43 GPa Show Material materials with Shear modulus of 60.43 GPa | |

550.0 °C | 58.76 GPa Show Material materials with Shear modulus of 58.76 GPa | |

600.0 °C | 57.09 GPa Show Material materials with Shear modulus of 57.09 GPa | |

650.0 °C | 55.43 GPa Show Material materials with Shear modulus of 55.43 GPa | |

700.0 °C | 53.86 GPa Show Material materials with Shear modulus of 53.86 GPa | |

750.0 °C | 52.29 GPa Show Material materials with Shear modulus of 52.29 GPa | |

800.0 °C | 50.72 GPa Show Material materials with Shear modulus of 50.72 GPa | |

Unlock all property charts | ||

Yield strength Rp0.2 | 20.0 °C | 255 MPa Show Material materials with Yield strength Rp0.2 of 255 MPa |

50.0 °C | 239 MPa Show Material materials with Yield strength Rp0.2 of 239 MPa | |

100.0 °C | 215 MPa Show Material materials with Yield strength Rp0.2 of 215 MPa | |

200.0 °C | 196 MPa Show Material materials with Yield strength Rp0.2 of 196 MPa | |

300.0 °C | 177 MPa Show Material materials with Yield strength Rp0.2 of 177 MPa | |

400.0 °C | 167 MPa Show Material materials with Yield strength Rp0.2 of 167 MPa | |

500.0 °C | 157 MPa Show Material materials with Yield strength Rp0.2 of 157 MPa | |

550.0 °C | 152 MPa Show Material materials with Yield strength Rp0.2 of 152 MPa | |

Unlock all property charts | ||

Yield strength Rp0.2, transverse | 20.0 °C | 255 MPa Show Material materials with Yield strength Rp0.2, transverse of 255 MPa |

Yield strength Rp1.0 | 20.0 °C | 295 MPa Show Material materials with Yield strength Rp1.0 of 295 MPa |

50.0 °C | 273 MPa Show Material materials with Yield strength Rp1.0 of 273 MPa | |

100.0 °C | 245 MPa Show Material materials with Yield strength Rp1.0 of 245 MPa | |

200.0 °C | 226 MPa Show Material materials with Yield strength Rp1.0 of 226 MPa | |

300.0 °C | 206 MPa Show Material materials with Yield strength Rp1.0 of 206 MPa | |

400.0 °C | 196 MPa Show Material materials with Yield strength Rp1.0 of 196 MPa | |

500.0 °C | 186 MPa Show Material materials with Yield strength Rp1.0 of 186 MPa | |

550.0 °C | 181 MPa Show Material materials with Yield strength Rp1.0 of 181 MPa | |

Unlock all property charts | ||

Yield strength Rp1.0, transverse | 20.0 °C | 295 MPa Show Material materials with Yield strength Rp1.0, transverse of 295 MPa |

Thermal

Property | Temperature | Value | Comment |
---|---|---|---|

Coefficient of thermal expansion | -100.0 °C | 1.49E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.49E-5 1/K | |

20.0 °C | 1.61E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.61E-5 1/K | ||

100.0 °C | 1.63E-5 - 1.67E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.63E-5 - 1.67E-5 1/K | ||

200.0 °C | 1.69E-5 - 1.72E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.69E-5 - 1.72E-5 1/K | ||

300.0 °C | 1.73E-5 - 1.77E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.73E-5 - 1.77E-5 1/K | ||

400.0 °C | 1.78E-5 - 1.81E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.78E-5 - 1.81E-5 1/K | ||

500.0 °C | 1.82E-5 - 1.84E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.82E-5 - 1.84E-5 1/K | ||

600.0 °C | 1.85E-5 - 1.88E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.85E-5 - 1.88E-5 1/K | ||

700.0 °C | 1.91E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.91E-5 1/K | ||

800.0 °C | 1.94E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.94E-5 1/K | ||

900.0 °C | 1.97E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.97E-5 1/K | ||

1000.0 °C | 2E-5 1/K Show Material materials with Coefficient of thermal expansion of 2E-5 1/K | ||

Unlock all property charts | |||

Max service temperature, long | 0 - 750 °C Show Material materials with Max service temperature, long of 0 - 750 °C | ||

Melting point | 1230 - 1480 °C Show Material materials with Melting point of 1230 - 1480 °C | Typical for Austenitic Stainless Steel | |

Specific heat capacity | -100.0 °C | 440 J/(kg·K) Show Material materials with Specific heat capacity of 440 J/(kg·K) | |

20.0 °C | 450 - 472 J/(kg·K) Show Material materials with Specific heat capacity of 450 - 472 J/(kg·K) | ||

100.0 °C | 487 J/(kg·K) Show Material materials with Specific heat capacity of 487 J/(kg·K) | ||

200.0 °C | 503 J/(kg·K) Show Material materials with Specific heat capacity of 503 J/(kg·K) | ||

300.0 °C | 512 J/(kg·K) Show Material materials with Specific heat capacity of 512 J/(kg·K) | ||

400.0 °C | 520 J/(kg·K) Show Material materials with Specific heat capacity of 520 J/(kg·K) | ||

500.0 °C | 530 J/(kg·K) Show Material materials with Specific heat capacity of 530 J/(kg·K) | ||

600.0 °C | 541 J/(kg·K) Show Material materials with Specific heat capacity of 541 J/(kg·K) | ||

700.0 °C | 551 J/(kg·K) Show Material materials with Specific heat capacity of 551 J/(kg·K) | ||

800.0 °C | 559 J/(kg·K) Show Material materials with Specific heat capacity of 559 J/(kg·K) | ||

900.0 °C | 565 J/(kg·K) Show Material materials with Specific heat capacity of 565 J/(kg·K) | ||

1000.0 °C | 571 J/(kg·K) Show Material materials with Specific heat capacity of 571 J/(kg·K) | ||

Unlock all property charts | |||

Thermal conductivity | 20.0 °C | 13.3 - 15 W/(m·K) Show Material materials with Thermal conductivity of 13.3 - 15 W/(m·K) | |

100.0 °C | 14.9 W/(m·K) Show Material materials with Thermal conductivity of 14.9 W/(m·K) | ||

200.0 °C | 16.5 W/(m·K) Show Material materials with Thermal conductivity of 16.5 W/(m·K) | ||

300.0 °C | 18.1 W/(m·K) Show Material materials with Thermal conductivity of 18.1 W/(m·K) | ||

400.0 °C | 19.5 W/(m·K) Show Material materials with Thermal conductivity of 19.5 W/(m·K) | ||

500.0 °C | 21 W/(m·K) Show Material materials with Thermal conductivity of 21 W/(m·K) | ||

600.0 °C | 22.4 W/(m·K) Show Material materials with Thermal conductivity of 22.4 W/(m·K) | ||

700.0 °C | 23.8 W/(m·K) Show Material materials with Thermal conductivity of 23.8 W/(m·K) | ||

800.0 °C | 25.2 W/(m·K) Show Material materials with Thermal conductivity of 25.2 W/(m·K) | ||

Unlock all property charts | |||

Thermal diffusivity | 20.0 °C | 3.5 mm²/s Show Material materials with Thermal diffusivity of 3.5 mm²/s | |

100.0 °C | 3.8 mm²/s Show Material materials with Thermal diffusivity of 3.8 mm²/s | ||

200.0 °C | 4 mm²/s Show Material materials with Thermal diffusivity of 4 mm²/s | ||

300.0 °C | 4.3 mm²/s Show Material materials with Thermal diffusivity of 4.3 mm²/s | ||

400.0 °C | 4.5 mm²/s Show Material materials with Thermal diffusivity of 4.5 mm²/s | ||

500.0 °C | 4.7 mm²/s Show Material materials with Thermal diffusivity of 4.7 mm²/s | ||

600.0 °C | 4.8 mm²/s Show Material materials with Thermal diffusivity of 4.8 mm²/s | ||

700.0 °C | 5.1 mm²/s Show Material materials with Thermal diffusivity of 5.1 mm²/s | ||

800.0 °C | 5.4 mm²/s Show Material materials with Thermal diffusivity of 5.4 mm²/s | ||

Unlock all property charts |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical resistivity | 20.0 °C | 7.9E-7 - 7.91E-7 Ω·m Show Material materials with Electrical resistivity of 7.9E-7 - 7.91E-7 Ω·m |

50.0 °C | 8.13E-7 Ω·m Show Material materials with Electrical resistivity of 8.13E-7 Ω·m | |

100.0 °C | 8.45E-7 Ω·m Show Material materials with Electrical resistivity of 8.45E-7 Ω·m | |

150.0 °C | 8.87E-7 Ω·m Show Material materials with Electrical resistivity of 8.87E-7 Ω·m | |

200.0 °C | 9.19E-7 Ω·m Show Material materials with Electrical resistivity of 9.19E-7 Ω·m | |

250.0 °C | 9.46E-7 Ω·m Show Material materials with Electrical resistivity of 9.46E-7 Ω·m | |

300.0 °C | 9.77E-7 Ω·m Show Material materials with Electrical resistivity of 9.77E-7 Ω·m | |

350.0 °C | 1E-6 Ω·m Show Material materials with Electrical resistivity of 1E-6 Ω·m | |

400.0 °C | 1.03E-6 Ω·m Show Material materials with Electrical resistivity of 1.03E-6 Ω·m | |

450.0 °C | 1.05E-6 Ω·m Show Material materials with Electrical resistivity of 1.05E-6 Ω·m | |

500.0 °C | 1.08E-6 Ω·m Show Material materials with Electrical resistivity of 1.08E-6 Ω·m | |

550.0 °C | 1.1E-6 Ω·m Show Material materials with Electrical resistivity of 1.1E-6 Ω·m | |

600.0 °C | 1.12E-6 Ω·m Show Material materials with Electrical resistivity of 1.12E-6 Ω·m | |

650.0 °C | 1.13E-6 Ω·m Show Material materials with Electrical resistivity of 1.13E-6 Ω·m | |

700.0 °C | 1.15E-6 Ω·m Show Material materials with Electrical resistivity of 1.15E-6 Ω·m | |

750.0 °C | 1.17E-6 Ω·m Show Material materials with Electrical resistivity of 1.17E-6 Ω·m | |

800.0 °C | 1.18E-6 Ω·m Show Material materials with Electrical resistivity of 1.18E-6 Ω·m | |

Unlock all property charts |

Chemical properties

Property | Value |
---|---|

Carbon | 0.04 - 0.1 % Show Material materials with Carbon of 0.04 - 0.1 % |

Chromium | 15.5 - 17.5 % Show Material materials with Chromium of 15.5 - 17.5 % |

Manganese | 1.5 % Show Material materials with Manganese of 1.5 % |

Molybdenum | 1.1 - 1.5 % Show Material materials with Molybdenum of 1.1 - 1.5 % |

Nickel | 12.5 - 14.5 % Show Material materials with Nickel of 12.5 - 14.5 % |

Niobium | 1.2 % Show Material materials with Niobium of 1.2 % |

Nitrogen | 0.06 - 0.14 % Show Material materials with Nitrogen of 0.06 - 0.14 % |

Phosphorus | 0.04 % Show Material materials with Phosphorus of 0.04 % |

Silicon | 0.3 - 0.6 % Show Material materials with Silicon of 0.3 - 0.6 % |

Sulfur | 0.015 % Show Material materials with Sulfur of 0.015 % |

Vanadium | 0.6 - 0.85 % Show Material materials with Vanadium of 0.6 - 0.85 % |